Download presentation

Presentation is loading. Please wait.

1
Quantum phase transitions: from Mott insulators to the cuprate superconductors Colloquium article in Reviews of Modern Physics 75, 913 (2003) Talk online: Sachdev

2
Outline A.“Dimerized” Mott insulators Landau-Ginzburg-Wilson (LGW) theory B.Mott insulators with spin S=1/2 per unit cell Berry phases, bond order, and the breakdown of the LGW paradigm C.Cuprate Superconductors Competing orders and recent experiments

3
“Dimerized” Mott insulators: Landau-Ginzburg-Wilson (LGW) theory: Second-order phase transitions described by fluctuations of an order parameter associated with a broken symmetry

4
TlCuCl 3 M. Matsumoto, B. Normand, T.M. Rice, and M. Sigrist, cond-mat/0309440.

5
TlCuCl 3 M. Matsumoto, B. Normand, T.M. Rice, and M. Sigrist, cond-mat/0309440.

6
S=1/2 spins on coupled dimers Coupled Dimer Antiferromagnet M. P. Gelfand, R. R. P. Singh, and D. A. Huse, Phys. Rev. B 40, 10801-10809 (1989). N. Katoh and M. Imada, J. Phys. Soc. Jpn. 63, 4529 (1994). J. Tworzydlo, O. Y. Osman, C. N. A. van Duin, J. Zaanen, Phys. Rev. B 59, 115 (1999). M. Matsumoto, C. Yasuda, S. Todo, and H. Takayama, Phys. Rev. B 65, 014407 (2002).

7
Weakly coupled dimers Paramagnetic ground state

8
Weakly coupled dimers Excitation: S=1 triplon

9
Weakly coupled dimers Excitation: S=1 triplon

10
Weakly coupled dimers Excitation: S=1 triplon Energy dispersion away from antiferromagnetic wavevector (exciton, spin collective mode)

11
TlCuCl 3 N. Cavadini, G. Heigold, W. Henggeler, A. Furrer, H.-U. Güdel, K. Krämer and H. Mutka, Phys. Rev. B 63 172414 (2001). “triplon” or spin exciton

12
S=1/2 spins on coupled dimers Coupled Dimer Antiferromagnet M. P. Gelfand, R. R. P. Singh, and D. A. Huse, Phys. Rev. B 40, 10801-10809 (1989). N. Katoh and M. Imada, J. Phys. Soc. Jpn. 63, 4529 (1994). J. Tworzydlo, O. Y. Osman, C. N. A. van Duin, J. Zaanen, Phys. Rev. B 59, 115 (1999). M. Matsumoto, C. Yasuda, S. Todo, and H. Takayama, Phys. Rev. B 65, 014407 (2002).

13
Square lattice antiferromagnet Experimental realization: Ground state has long-range magnetic (Neel or spin density wave) order Excitations: 2 spin waves (magnons)

14
TlCuCl 3 J. Phys. Soc. Jpn 72, 1026 (2003)

15
1 Neel state T=0 Pressure in TlCuCl 3 Quantum paramagnet c = 0.52337(3) M. Matsumoto, C. Yasuda, S. Todo, and H. Takayama, Phys. Rev. B 65, 014407 (2002) The method of bond operators (S. Sachdev and R.N. Bhatt, Phys. Rev. B 41, 9323 (1990)) provides a quantitative description of spin excitations in TlCuCl 3 across the quantum phase transition (M. Matsumoto, B. Normand, T.M. Rice, and M. Sigrist, Phys. Rev. Lett. 89, 077203 (2002))

16
LGW theory for quantum criticality ~3 Three triplon continuum Triplon pole Structure holds to all orders in u A.V. Chubukov, S. Sachdev, and J.Ye, Phys. Rev. B 49, 11919 (1994) S. Chakravarty, B.I. Halperin, and D.R. Nelson, Phys. Rev. B 39, 2344 (1989)

17
Mott insulators with spin S=1/2 per unit cell: Berry phases, bond order, and the breakdown of the LGW paradigm

18
Mott insulator with two S=1/2 spins per unit cell

19
Mott insulator with one S=1/2 spin per unit cell

21
Destroy Neel order by perturbations which preserve full square lattice symmetry e.g. second-neighbor or ring exchange

22
Mott insulator with one S=1/2 spin per unit cell Destroy Neel order by perturbations which preserve full square lattice symmetry e.g. second-neighbor or ring exchange

23
Mott insulator with one S=1/2 spin per unit cell

34
Resonating valence bonds Resonance in benzene leads to a symmetric configuration of valence bonds (F. Kekulé, L. Pauling) The paramagnet on the square lattice should also allow other valence bond pairings, and this implies a “resonating valence bond liquid” with =0 (P.W. Anderson, 1987)

35
Quantum theory for destruction of Neel order Ingredient missing from LGW theory: Spin Berry Phases

36
Quantum theory for destruction of Neel order Ingredient missing from LGW theory: Spin Berry Phases

37
Discretize imaginary time: path integral is over fields on the sites of a cubic lattice of points a Quantum theory for destruction of Neel order

38
Partition function on cubic lattice Modulus of weights in partition function: those of a classical ferromagnet at “temperature” g Quantum theory for destruction of Neel order

40
Change in choice of n 0 is like a “gauge transformation” ( a is the oriented area of the spherical triangle formed by n a and the two choices for n 0 ). The area of the triangle is uncertain modulo 4 and the action is invariant under These principles strongly constrain the effective action for A a which provides description of the large g phase

41
Simplest large g effective action for the A a S. Sachdev and R. Jalabert, Mod. Phys. Lett. B 4, 1043 (1990). S. Sachdev and K. Park, Annals of Physics 298, 58 (2002).

42
N. Read and S. Sachdev, Phys. Rev. Lett. 62, 1694 (1989).

43
For large e 2, low energy height configurations are in exact one-to- one correspondence with nearest-neighbor valence bond pairings of the sites square lattice There is no roughening transition for three dimensional interfaces, which are smooth for all couplings There is a definite average height of the interface Ground state has bond order. N. Read and S. Sachdev, Phys. Rev. Lett. 62, 1694 (1989).

44
Smooth interface with average height 3/8 W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) 0 0 1/2 1/4 3/4

45
W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) Smooth interface with average height 5/8 1 1 1/2 1/4 3/4

46
Smooth interface with average height 7/8 W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) 1 1 1/2 5/4 3/4

47
Smooth interface with average height 1/8 W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) 0 0 1/2 1/4 -1/4

48
“Disordered-flat” interface with average height 1/2 1/2 1/4 3/4 W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) 1/4 3/4

49
“Disordered-flat” interface with average height 3/4 1/2 3/4 W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) 1 1 1 1 3/4

50
1/4 -1/4 W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) 0 1/4 0 0 0 -1/4 “Disordered-flat” interface with average height 0

51
1/4 W. Zheng and S. Sachdev, Phys. Rev. B 40, 2704 (1989) 0 “Disordered-flat” interface with average height 1/4 1/2 1/4 0 0 0

52
g 0 ? or

53
A. W. Sandvik, S. Daul, R. R. P. Singh, and D. J. Scalapino, Phys. Rev. Lett. 89, 247201 (2002) Bond order in a frustrated S=1/2 XY magnet g= First large scale numerical study of the destruction of Neel order in a S=1/2 antiferromagnet with full square lattice symmetry

54
g 0 ? or

55
Naïve approach: add bond order parameter to LGW theory “by hand” g g First order transition g

56
g 0 S. Sachdev and R. Jalabert, Mod. Phys. Lett. B 4, 1043 (1990). S. Sachdev and K. Park, Annals of Physics 298, 58 (2002). ? or

57
T. Senthil, A. Vishwanath, L. Balents, S. Sachdev and M.P.A. Fisher, Science, March 5, 2004 Theory of a second-order quantum phase transition between Neel and bond-ordered phases Second-order critical point described by emergent fractionalized degrees of freedom (A and z ); Order parameters ( and ) are “composites” and of secondary importance

58
g Phase diagram of S=1/2 square lattice antiferromagnet T. Senthil, A. Vishwanath, L. Balents, S. Sachdev and M.P.A. Fisher, Science, March 5, 2004 or

59
Cuprate superconductors: Competing orders and recent experiments

60
g one Main idea: one of the effects of doping mobile carriers is to increase the value of g States with co-existence of bond order and d-wave superconductivity S. Sachdev and N. Read, Int. J. Mod. Phys. B 5, 219 (1991). M. Vojta and S. Sachdev, Phys. Rev. Lett. 83, 3916 (1999); M. Vojta, Phys. Rev. B 66, 104505 (2002). Magnetic, bond and super- conducting order La 2 CuO 4 or

61
J. M. Tranquada, H. Woo, T. G. Perring, H. Goka, G. D. Gu, G. Xu, M. Fujita, and K. Yamada, cond-mat/0401621 Neutron scattering measurements of La 1.875 Ba 0.125 CuO 4 (Zurich oxide) Spin density wave of 8 lattice spacings along the principal square lattice axes Possible microscopic picture Bragg diffraction off static spin order

62
J. M. Tranquada, H. Woo, T. G. Perring, H. Goka, G. D. Gu, G. Xu, M. Fujita, and K. Yamada, cond-mat/0401621 Neutron scattering measurements of La 1.875 Ba 0.125 CuO 4 (Zurich oxide) Spin density wave of 8 lattice spacings along the principal square lattice axes Possible microscopic picture Bragg diffraction off static spin order with multiple domains

63
J. M. Tranquada, H. Woo, T. G. Perring, H. Goka, G. D. Gu, G. Xu, M. Fujita, and K. Yamada, cond-mat/0401621 Neutron scattering measurements of La 1.875 Ba 0.125 CuO 4 (Zurich oxide) Spin density wave of 8 lattice spacings along the principal square lattice axes Possible microscopic picture Bragg diffraction off static spin order with multiple domains (after rotation by 45 o )

64
At higher energies, expect “spin-wave cones”. Only seen at relatively low energies.

65
Proposal of J. M. Tranquada et al., cond-mat/0401621 High energy spectrum is the triplon excitation of two-leg spin ladders presence of bond order

66
Proposal of J. M. Tranquada et al., cond-mat/0401621 High energy spectrum is the triplon excitation of two-leg spin ladders presence of bond order

67
Proposal of J. M. Tranquada et al., cond-mat/0401621 Location of maximum energy excitations Superposition and rotation by 45 degrees High energy spectrum is the triplon excitation of two-leg spin ladders presence of bond order

68
Computation from isolated 2 leg ladders J. M. Tranquada et al., cond-mat/0401621

69
La 1.875 Ba 0.125 CuO 4 YBa 2 Cu 3 O 6.85

70
Understanding spectrum at all energies requires coupling between ladders, just past the quantum critical point to the onset of long-range magnetic order M. Vojta and T. Ulbricht, cond-mat/0402377 Use bond-operator method (S. Sachdev and R.N. Bhatt, Phys. Rev. B 41, 9323 (1990)) to compute crossover from spin-waves at low energies to triplons at high energies

71
M. Vojta and T. Ulbricht, cond-mat/0402377J. M. Tranquada et al., cond-mat/0401621 Possible evidence for spontaneous bond order in a doped cuprate

72
100Å b 7 pA 0 pA Vortex-induced LDOS of Bi 2 Sr 2 CaCu 2 O 8+ integrated from 1meV to 12meV J. Hoffman E. W. Hudson, K. M. Lang, V. Madhavan, S. H. Pan, H. Eisaki, S. Uchida, and J. C. Davis, Science 295, 466 (2002). Our interpretation: STM evidence for fluctuating spin density/bond order pinned by vortices/impurities A. Polkovnikov, S. Sachdev, M. Vojta, and E. Demler, Int. J. Mod. Phys. B 16, 3156 (2002)

73
Our interpretation: STM evidence for fluctuating spin density/bond order pinned by vortices/impurities A. Polkovnikov, S. Sachdev, M. Vojta, and E. Demler, Int. J. Mod. Phys. B 16, 3156 (2002) C. Howald, H. Eisaki, N. Kaneko, M. Greven,and A. Kapitulnik, Phys. Rev. B 67, 014533 (2003). STM image of LDOS modulations (after filtering in Fourier space) in Bi 2 Sr 2 CaCu 2 O 8+ in zero magnetic field

74
Our interpretation: STM evidence for fluctuating spin density/bond order pinned by vortices/impurities A. Polkovnikov, S. Sachdev, M. Vojta, and E. Demler, Int. J. Mod. Phys. B 16, 3156 (2002) LDOS of Bi 2 Sr 2 CaCu 2 O 8+ at 100 K. M. Vershinin, S. Misra, S. Ono, Y. Abe, Y. Ando, and A. Yazdani, Science, 12 Feb 2004.

75
Our interpretation: STM evidence for fluctuating spin density/bond order pinned by vortices/impurities A. Polkovnikov, S. Sachdev, M. Vojta, and E. Demler, Int. J. Mod. Phys. B 16, 3156 (2002) Energy integrated LDOS (between 65 and 150 meV) of strongly underdoped Bi 2 Sr 2 CaCu 2 O 8+ at low temperatures, showing only regions without superconducting “coherence peaks” K. McElroy, D.-H. Lee, J. E. Hoffman, K. M. Lang, J. Lee, E. W. Hudson, H. Eisaki, S. Uchida, and J.C. Davis, cond-mat/0402xxx.

76
Conclusions I.Theory of quantum phase transitions between magnetically ordered and paramagnetic states of Mott insulators: A. Dimerized Mott insulators: Landau-Ginzburg- Wilson theory of fluctuating magnetic order parameter. B. S=1/2 square lattice: Berry phases induce bond order, and LGW theory breaks down. Critical theory is expressed in terms of emergent fractionalized modes, and the order parameters are secondary. II. Preliminary evidence for spin density/bond orders in superconducting cuprates Conclusions I.Theory of quantum phase transitions between magnetically ordered and paramagnetic states of Mott insulators: A. Dimerized Mott insulators: Landau-Ginzburg- Wilson theory of fluctuating magnetic order parameter. B. S=1/2 square lattice: Berry phases induce bond order, and LGW theory breaks down. Critical theory is expressed in terms of emergent fractionalized modes, and the order parameters are secondary. II. Preliminary evidence for spin density/bond orders in superconducting cuprates

Similar presentations

© 2019 SlidePlayer.com Inc.

All rights reserved.

To make this website work, we log user data and share it with processors. To use this website, you must agree to our Privacy Policy, including cookie policy.

Ads by Google